Presentation on theme: "Soft bend elastic constant and transition to a modulated nematic phase Alenka Mertelj, 1 Martin Čopič, 1,* Geoffrey R. Luckhurst 2, R. P. Tuffin 3, and."— Presentation transcript:
Soft bend elastic constant and transition to a modulated nematic phase Alenka Mertelj, 1 Martin Čopič, 1,* Geoffrey R. Luckhurst 2, R. P. Tuffin 3, and Owain Parri 3 1 Faculty of Mathematics and Physics, University of Ljubljana, Jadranska 19, Ljubljana 1000, Slovenia 2 School of Chemistry, University of Southampton, Southampton SO17 1BJ, UK 3 Merck Chemicals Ltd, Chilworth Technical Centre, University Parkway, Southampton SO16 7QD, UK
Outline Observation of modulated phase in nematic phase of flexible dimers Nematic fluctuations and dynamic light scattering Temperature and order parameter dependence of elastic constants Conclusions
Modulated nematic phase Observed in flexible dimers of biphenyls like 1,7-bis(4-cyanobiphenyl-4-yl)heptane (CB7CB) and CB9CB , or CB11CB I.Dozov  proposed that a softening of the bend elastic constant could lead to a modulated nematic phase with nematic director forming a twist-bend helix In  it was suggested that in CB11CB the modulation is due to soft splay elastic constant Numerical modeling of A. Ferrarini indicates that bend elastic constant in dimers can become negative  M. Cestari et al., Phys. Rev. E 84, 031704 (2011)  V. P. Panov et al., Phys. Rev. Lett.105, 167801 (2010).  I. Dozov, Europhys. Lett. 56, 24 (2001).
Light scattering Elastic constants can be measured by observation of thermal director flucutations Relaxation rates give ratios K i /η i Scattering intensity gives ( ε) 2 /K i As ε is proportional to S, we get K i /S 2 K i /S 2 are lowest order “bare” elastic coefficients in Landau-deGennes free energy
Relaxation rates Two modes: bend-splay and bend-twist, for q along n – pure bend Relaxation rates: Effective viscosities: Usually α 2 >> α 3, so that bend viscosity is smaller due to backflow The direction and polarization of the incoming and scattered light and n determine which mode is observed
Samples NC(CH 2 ) x CN X=7,9 - CB7CB and CB9CB CB7CB : T NI = 116 o C, T NX = 103 o C CB9CB : T NI = 124 o C, T NX = 109 o C Planar orientation
CB7CB diffusivities (K/η) Note increase in the splay diffusivity below T NX
CB9CB diffusivities (K/η) Note increase in the splay diffusivity below T NX
Normalized “bare” elastic constants CB7CBCB9CB Absolute scattering cross-sections is difficult to measure, so we obtain only T dependence of K i relative to the value at T NI The bend constant softens, but increases just above T NX The splay constant increases below T NX, also seen in diffusivity
“Bare” elastic constants – linear scale CB7CB CB9CB K i are normalized to 1 at T NI.
CB9CB: True K 3 The increase close to T NI is due to S 2 Δn measured by polarization interference Δn is proportional to S
True elastic constants of CB9CB. Values are relative to the values at TNI. Black squares - splay, green triangles – twist, red circles – bend.
Mixture of dimers The phase diagram for a mixture of KA and the liquid crystal dimer, CBF9CBF
Elastic constants of mixture by Frederiks transition Minimum K 3 =0.63 pN – by light scattering 0.3 pN
Relation to cubic invariants To quadratic order in gradient of Q splay and bend constants are equal. Cubic invariants that contribute to the elastic constants are
Values of third order coefficients Ki/S2 as functions of Δn for CB7CB (left) and CB9CB (right). C 1 negative, C 2 and C 3 about 0 Transition seems to be driven by increase in S
Problems Bend constant increases just before the transition to Nx phase –Bent core molecules also have small bend constant, but go to Sm phase – perhaps the increase of K 3 due to competition with smectic order Standard methods based on Frederiks transition give smaller decrease of the bend constant
Conclusions Bend elastic constant in the nematic phase of flexible dimers dramatically decreases with T and is probably the cause of an instability resulting in the modulated phase Just above the transition K 3 slightly increases – effect of pretransitional fluctuations? Below the transition light scattering corresponding to splay fluctuations strongly decreases – analogy with SmA phase?